Novel TiO2 Photocatalyst Using Nonaqueous Solvent- Controlled Sol-Gel Route

Synthesis of metal oxide nanoparticles with tailored properties is of great interest because of their potential in environmental, sensor, biomedical and energy applications. Specifically, TiO 2 gets special attention because of its high stability, biocompatibility, tunable band gap and surface properties. Aqueous sol-gel routes for the synthesis of TiO 2 nanoparticles are well established but suffer from little control over morphology and reproducibility. Nonaqueous solvent controlled sol-gel routes are good alternative to aqueous routes for the synthesis of highly crystalline TiO 2 nanoparticles with high purity and controlled doping of large size metallic ions. Present chapter describes the successful doping of large sized Zr and Na metal ions at Ti site and their influence on photo catalytic activity of TiO 2 . The higher photo catalytic activity (even better than commercially available Degussa P25) of metal doped TiO 2 nanopowder is attributed to large surface area and reduced electron-hole recombination rate.


Introduction
Metal oxide nanoparticles (MONPs) are well-known for their outstanding role especially for environmental, sensor, biomedical and energy applications [1][2][3][4][5][6][7][8][9][10]. Among MONPs, TiO 2 nanoparticles are least toxic [11] and therefore synthesis of nanostructured TiO 2 with tailored properties has been most extensively investigated in recent years.TiO 2 occurs in three different phases [12], anatase, rutile and brookite with rutile as most stable phase and anatase as most desirable phase. TiO 2 is associated with outstanding properties including high stability, A large number of synthesis methods have been employed for designing of TiO 2 nanoparticles with controlled shape, size, good yield and high dispersibility (less agglomeration). The shape and size of nanoparticles greatly affect the photocatalytic performance of the photocatalyst [26,27]. Highly pure metal oxides can be prepared by conventional solid state route [28], but high processing temperature requirement limits its frequent use for synthesis. The biological synthesis method [11,29] leads to formation of cost-effective, mono-dispersed nanoparticles but reproducibility needs improvement. To overcome all these difficulties during nanoparticles synthesis, alternative well-known liquid phase synthesis methods such as sol-gel [30,31], hydrothermal [32,33], microemulsion [34,35], reverse microemulsion [36], sonochemical [37,38] and microwave [39,40] are employed. Among these synthesis methods, the sol-gel synthesis route gets special attention because of following reasons: general results in amorphous powder after drying process. The process of mixing is known as hydrolysis, while formation of 3-dimensional network is called as condensation. These two processes are further controlled by many parameters including nature of metal precursor, ratio of precursor to solvent, nature of solvent, capping agents (surfactants), pH and temperature. Figure 1 summarizes the various types of sol-gel routes.
Aqueous sol-gel route [41], as its name suggests, uses water as solvent to dissolve metal precursor and to complete hydrolysis process. The hydrolysis process is extremely fast due to high reactivity of water with precursors and therefore, generally there is little control over morphology and reproducibility. Nonaqueous sol-gel routes offer a good alternative to get rid of these difficulties [43,44]. An organic solvent (alcohols, ketones, aldehydes or ethers) is used to complete the hydrolysis process instead of water. Besides, the oxygen required for metal-oxide formation is supplied by organic solvent in nonaqueous sol-gel route, whereas water plays the role of oxygen donor in aqueous sol-gel synthesis. However, inclusion or exclusion of some surfactant (consisting of hydrophilic and hydrophobic groups) in reaction solution further classifies the nonaqueous sol-gel route into surfactant assisted and solvent controlled (surfactant free) routes respectively. The main advantage of surfactant assisted nonaqueous sol-gel route is that the surfactant acts as capping agent and results in highly mono-dispersed nanoparticles. In addition a good control over particle size, morphology with outstanding reproducibility is direct consequence of surfactant-assisted nonaqueous sol-gel route. Moreover, the surface properties of nanoparticles can be easily tailored by exchanging surfactants with other functional groups. However this method is also prone to certain limitations like impurities in nanoparticles and toxic effects due to surfactants. These limitations impose restrictions on the surface sensitive applications (photocatalytic, biomedical and sensing) of nanoparticles.

Solvent controlled nonaqueous sol-gel route
A good alternative to surfactant assisted nonaqueous sol-gel route [45,46] is solvent controlled nonaqueous sol-gel route. The solvent in itself plays role of oxygen donor necessary for oxide formation and stabilizing agent to control shape, size and morphology of nanoparticles. This modified sol-gel route also facilitates highly pure nanoparticles completely free  from toxic surfactants but suffers from tendency to agglomerate. However toxic effect of halides cannot be neglected when metal oxide nanoparticles are prepared by reacting metal halides with organic solvents. In order to avoid halide impurities from metal oxide nanoparticles it is wise to use metal alkoxides, acetates or acetylacetonates as metal precursor. In the following subsections, synthesis of pristine and metal doped TiO 2 nanoparticles using halide free, nonaqueous, solvent controlled sol-gel route [2, 10] is described.

Synthesis of pristine TiO 2
Titanium tetra iso-propoxide (TTIP) was used as Titanium precursor and methoxyethanol as organic solvent. 20 ml TTIP is added to 40 ml methoxyethanol and mixed using magnetic stirrer. The pH of solution is adjusted to value 3 using 1 M HNO 3 , which also catalyzes the hydrolysis process. The mixing is continued until viscous gel is formed, which is then dried under IR lamp and pulverized to obtain amorphous powder. The pure anatase TiO 2 nanopowder is formed after calcining the amorphous powder at 450°C for 1 hour. The chemical reactions occurring during hydrolysis and condensation in the synthesis are listed below.

Synthesis of metal doped TiO 2
What is the motivation for metal doping in TiO 2 ? As explained earlier, TiO 2 is wide band gap semiconductor and requires UV irradiation for its operation as a photo catalyst. The contribution of UV light in the solar radiation is less than 5%. Therefore, it is required to tune the band gap of TiO 2 to visible range so that no extra source of radiation energy (other than solar light) is required. Also, pristine TiO 2 suffers from higher recombination rate of charge carriers (electron and hole) resulting in less photocatalytic efficiency. Metals [10,[47][48][49][50][51][52] and nonmetals [53][54][55][56][57][58] are well known for their ability to reduce the band gap of TiO 2 by generating energy states between valence band and conduction band. These energy states serve as charge carrier trapping center and therefore reduce the electron hole recombination rate. The reduction in electron hole recombination rate results in remarkable improvement in photocatalytic performance. In addition, noble metals (Ag, Au and Pt), transition metals [59][60][61] and nonmetals doping in TiO 2 reduces the band gap of TiO 2 to visible range. Moreover, many doped TiO 2 nanoparticles are found to have small size as compared to pristine TiO 2 , which improves the surface area and consequently boosts up the photocatalytic performance. However, favorable change in properties of TiO 2 by doping is largely affected by synthesis methods.
In current chapter, synthesis and photocatalytic properties of TiO 2 nanoparticles doped with one transition metal, Zirconium (Zr) and one other alkali metal, sodium (Na) are discussed. Both these metals have higher ionic radii (~0.79 Å for Zr and ~1.02 Å for Na) as compared to titanium (~0.68 Å for Ti). Large ionic radii and low valence ionic metallic dopant in host Ti4+ always results in strain in the crystal structure that favors the formation of oxygen vacancies [62]. These oxygen vacancies are prone to trap electrons and suppress grain growth resulting Titanium Dioxide -Material for a Sustainable Environment in reduced charge recombination rate and small crystallite size respectively. There are many reports which claimed contradictory reports on photocatalytic activity of TiO 2 after doping of same dopant under different synthesis routes. Bessekhouad et al. [63] compared the photo catalytic efficiency of Na doped TiO 2 nanopowder prepared via two methods: sol-gel route and impregnation technology. They found that photo catalytic efficiency of nanopowder prepared by impregnation technology is higher than nanopowder prepared by aqueous sol-gel route. In addition, Na doping in TiO 2 matrix via aqueous sol-gel route decreases the photocatalytic efficiency due to migration of Na at TiO 2 surface instead of entering in the lattice.
On the other hand, Yang et al. [64] showed higher photocatalytic activity of Na doped TiO 2 nanopowder prepared via solvothermal method. XRD analysis by Yang et al. [64], Xie et al.
[65] as well as Bessekhouad et al. [63] could not confirm the doping of large sized Na into TiO 2 lattice and therefore hinted at the tendency of large sized Na + ions to migrate to TiO 2 surface. Therefore, it is required to study the effect of synthesis method on doping mechanism and photocatalytic activity of large sized metal dopants in TiO 2 matrix.
In [2,10] Zr and Na has been doped in TiO 2 matrix individually by solvent controlled nonaqueous sol-gel route. Easily dissolvable zirconium oxy-nitrate and sodium nitrate are used as precursor of Zr and Na respectively. To achieve nominal dopants concentration, calculated amount of precursor is added to solvent prior to addition of Ti precursor. After complete dissolution of dopant precursor, Ti precursor is added to reaction solution and similar steps are followed as in preparation of doped TiO 2 nanopowder.

Phase and structural characterization
X-ray diffraction (XRD) is an important tool used to determine the phase purity of sample, crystal structure, lattice parameter, average crystallite size and quantitative phase analysis. Generally, as prepared TiO 2 by sol-gel route is amorphous and therefore requires different heat treatment to form crystalline phases. Low (300-500°C), moderate (500-700°C) and high (more than 700°C) calcination temperature results in pure anatase phase, mixture of anatase and rutile, and pure rutile phase respectively [66]. The anatase to rutile (A-R) phase transformation is largely affected by type and amount of metal doping. Choi et al. [67] studied effect of single metal ion doping on A-R phase transformation temperature in TiO 2 prepared by sol-gel route. They observed that many metals such as Pt, Cr, V, Fe, La doping in TiO 2 lowers the A-R transformation temperature, whereas Ru metal shows opposite behavior. Xie et al. [65] and Singh et al. [2] also reported increased A-R transformation temperature in Na doped TiO 2 nanopowder. The presence of rutile structure in anatase phase affects the photocatalytic activity of metal doped TiO 2 . types of doping is favored, depends on size of guest ion as compared to host ion and volume size of interstitial position in the host lattice. Substitutional doping is preferred in case where size of guest ion is comparable or slightly larger than lattice ion, whereas if size of guest ion is much smaller than lattice ion then it occupies interstitial position of host lattice.
XRD peaks of crystal planes of Zr doped TiO 2 (Figure 2(A)) shows red shift in 2θ values, which confirms the substitutional doping of Zr 4+ at Ti 4+ site [10]. The substitutional doping of Zr in TiO 2 results in an increase in cell parameter and cell volume as reported by Yu et al. [68] and Wang et al. [69] Thus, incorporation of large sized Zr results in lattice strain and hence leads to formation of oxygen vacancies and suppresses the grain growth. Similar behavior is observed for Na doped TiO 2 nanopowder (Figure 2(B)) [2]. However formation of oxygen vacancies in Na doped TiO 2 can occur not only due to strain induced by Na doping but also due to lower valence state of Na +1 ion. It should be noted that there are contradictory literature reports regarding doping of Na in TiO 2 . Xie et al. [65] who used aqueous sol-gel synthesis, reported that large size Na cannot substitute Ti and therefore migrates to TiO 2 surface forming Na-O bonds as there is no peak shift is observed in XRD patterns. Thus it appears that substitutional doping of Na at Ti in TiO 2 , as indicated by the XRD peak shifts in Figure 2(B), is facilitated by nonaqueous solvent controlled sol-gel route, which was used by Singh et al. [10].
The crystallite size of pristine and doped TiO 2 nanopowder are calculated by well-known Debye Scherrer formula and tabulated in

Microstructural characterization
XRD gives structural information like lattice constant and crystalline phases averaged over bulk of the material. TEM on the other hand is able to give microstructural information on

Photoluminescence study
Photoluminescence (PL) spectroscopy is a versatile and powerful optical method to investigate the energy levels in materials. The material is irradiated with light photons of energy greater than or equal to band gap energy of material. This results in the excitation of electrons from valence band to the excited states (Figure 4(A)) of material. These electrons relax to conduction band by losing excess energy via nonradiative process. When these electrons return to their valence band, the energy is released in the form of photons and the process is known as photoluminescence. The energy of emitted photons is determined by the difference in atomic energy levels, while the intensity of emitted light gives us information regarding recombination of electrons and holes.
The energy and intensity of emitted light in PL spectra of particular material is highly affected by doping. Figure 4(B) shows the PL spectra of pristine and Na doped TiO 2 nanopowder at excitation wavelength 390 nm. The shape of PL signal remains same while intensity reduces with increase in doping concentration of Na in TiO 2 matrix. This is attributed to the fact that Na doping in TiO 2 matrix results in formation of oxygen vacancies resulting in energy states lying between valence band and conduction band that trap the electrons form conduction band and thereby reduce electron-hole recombination [68]. However, the PL signal intensity increases for Ti 0.9 Na 0.1 O 2 sample. This is attributed to fact that excessive formation of oxygen vacancies might act as recombination centers [70].

Photocatalytic activity
The photocatalytic activity of prepared photo catalyst can be measured by many different test methods [71], which have been accepted at national and international standards. We have used German standard DIN 52980 11 for the determination of photocatalytic activity. This standard Titanium Dioxide -Material for a Sustainable Environment method is based on the degradation of organic dye methylene blue (MB) by photo catalyst under UV irradiation. The degradation results are further confirmed by measuring total organic carbon (TOC) of initial dye aqueous solution and degraded dye aqueous solution by TOC analyzer.

Degradation experiment
The photocatalytic activity of pristine and metal doped TiO 2 is evaluated by degrading aqueous solution of MB dye under ultraviolet (UV) irradiation. In order to compare photocatalytic activity of photo catalyst prepared by nonaqueous solvent controlled sol-gel route with commercial photo catalyst, the photocatalytic activity of well-known commercially available Degussa P25 TiO 2 is also evaluated. The initial concentration of MB aqueous solution is 5 mg/L. About 100 ml of MB dye aqueous solution (pH 5) is taken in 100 ml borosil glass beaker and 60 mg of photo catalyst is added in the solution. The beaker is kept on magnetic stirrer for uniform suspension of photo catalyst in the solution throughout the experiment. The reaction mixture is irradiated by UV light of peak wavelength at 365 nm and the intensity of UV light at the surface of reaction mixture is 10 mW/cm 2 .
The distance between reaction mixture and UV light source is 20 cm resulting in light intensity of 8 × 10 4 lux over reaction mixture. In order to complete adsorption-desorption equilibrium between photo catalyst and dye, the reaction mixture is stirred for 20 minutes in completely dark chamber. After achieving adsorption-desorption equilibrium, the reaction mixture is irradiated with UV light and a small amount of solution is withdrawn at regular time intervals. The withdrawn sample is centrifuged to separate out nanoparticles from the solution and absorbance of supernatant measured using UV-Visible spectrometer. The photocatalytic degradation percentage of dye for different time intervals is plotted for several photo catalysts and without catalyst (WC).
The degradation percentage of dye is calculated using Eq. 1. The rate constant (k) for the photocatalytic degradation of dye is determined from pseudo first order law using Eq. 2.
where C 0 is dye concentration before UV irradiation and C t is dye concentration after t time of UV irradiation.
In order to further confirm the degradation results, TOC of irradiated and nonirradiated dye aqueous solution is measured and TOC removal rate percentage is calculated using Eq. 3.
where TOC 0 and TOC t are the TOC values of dye solution before and after time 't' of UV irradiation respectively.

Degradation results and mechanism
The photocatalytic activity of prepared Na doped TiO 2 photo catalyst can be compared from Figure 5.  [10] for which, in addition to reduction in crystallite size and electron-hole recombination, band gap was also reduced due to Zr doping.
The photocatalytic degradation of dye at the surface of TiO 2 is well explained in the existing literature [56,72].
O 2 ̅ + 2H + + e − = 2 OH * MB + OH * = Degradation products (8) In pristine TiO 2 the higher recombination rate of electron-hole results in fewer number of ROS radicals and hence less photocatalytic activity. In addition, large energy gap and small surface area also limit the degradation efficiency. Metal doping in TiO 2 results in large surface area, band gap tuning toward visible range and reduced electron-hole recombination rate. This most general proposed mechanism for degradation of dye at surface of metal doped TiO 2 is depicted in Figure 6.

Conclusion
In this chapter the importance of recently reported nonaqueous solvent controlled sol-gel route for the synthesis of metal doped TiO 2 with improved photocatalytic properties discussed. Pristine as well as Zr and Na doped TiO 2 nanoparticles have been prepared by this modified sol-gel route and their photocatalytic activity evaluated. Successful doping of these large metal ions in TiO 2 lattice using this synthesis route was confirmed by shifts in XRD peak positions and increase in d spacing observed from HRTEM images.
The photocatalytic activity of metal doped TiO 2 nanopowder is found to be much higher than pristine TiO 2 , and even superior to commercially available Degussa P25 TiO 2 photo catalyst. This is attributed to large surface area due to small grain size and reduced electron hole Novel TiO 2 Photocatalyst Using Nonaqueous Solvent-Controlled Sol-Gel Route http://dx.doi.org/10.5772/intechopen.74568 recombination due to formation of oxygen vacancies in metal doped TiO 2 . The reduction in electron-hole recombination increases the availability of electrons and holes which reacts with adsorbed oxygen and water molecules forming large number of reactive oxygen active species leading to enhanced photocatalytic activity.
In past years, only few MONPs have been prepared by this nonaqueous, solvent controlled, sol-gel route. This method has great potential to synthesize functional nanoparticles of desired composition, size and surface properties essential for different applications.